adsorption study of acid red 18 from aqueous solution on to activated carbon prepared from murraya koenigii (curry tree) seeds
Asian Journal of Chemistry; Vol. 23, No. 1 (2011), 219-224 Adsorption of Acid Red 18 from Aqueous Solution onto Activated Carbon Prepared from Murraya koenigii (Curry Tree) Seeds S. SURESH1,*, R. WILFRED SUGUMAR2 and T. MAIYALAGAN31 Department of Chemistry, Panimalar Institute of Technology, Chennai-602 103, India2 Department of Chemistry, Madras Christian College, Chennai-600 059, India3 South African Institute for Advanced Materials Chemistry, University of the Western Cape, Bellville 7535, Cape Town, South Africa*Corresponding author: E-mail: firstname.lastname@example.org (Received: 3 February 2010; Accepted: 25 August 2010) AJC-9024 This paper focuses on the adsorption of acid red 18 onto low cost adsorbent prepared from Murraya koenigii seeds (MKS) from aqueous solutions at room temperature (25 ºC). Batch experiments were conducted and the effect of different process parameters such as adsorbent dosage and initial dye concentration were studied. The adsorption isotherm data was analyzed using Langmuir, Freundlich and Temkin isotherm models. The equilibrium data fits well with Langmuir adsorption isotherm and the monolayer adsorption capacity was found to be 53.19 mg/g. The adsorption kinetics was studied using pseudo-first order and pseudo-second order models. The rate of adsorption was found to conform to pseudo-second order kinetics with a good correlation (R2 > 0.99). The activated carbon prepared was characterized by SEM and FT-IR spectra. The results prove that Murraya koenigii seeds is a good low cost adsorbent for the removal of acid red 18 from aqueous solution. Key Words: Activated carbon, Adsorption, Dye removal, Equilibrium, Kinetics. INTRODUCTION hulls16, agricultural wastes17 etc. The present work is to investi- gate the adsorption phenomenon using Murraya koenigii seed Dyes are widely used in textile, paper, leather, coir pith, as an adsorbent. The seed of Murraya koenigii or as it iscarpet and cosmetic industries. The textile industry is one of commonly known as curry tree seed is abundantly availablethe largest producers of industrial waste water. The effluent in south India and hence it is used as an adsorbent material forreleased from these industries, if not treated properly, is a major the removal of acid red 18 from aqueous solution.environmental concern. Effluents from the textile industry arehighly coloured and disposal of this coloured water into the EXPERIMENTALreceiving water body causes damage to aquatic life and human In this study a commercially available textile dyestuffbeings1,2. A lot of synthetic dyestuffs used in textile industry namely acid red 18 is used as adsorbate. The molecular structurewere found to be toxic, carcinogenic and even mutagenic3. and properties of acid red 18 is shown in Fig. 1 and Table-1,Thus the effluents need to be treated properly before being respectively. The dye is widely used in textile industries. Thereleased in to the environment. selected dyestuff is a dye contaminant in the discharged effluents There are several treatment methods like photo degradation4, commonly used in dye houses.coagulation, flocculation5 and electrochemical oxidation6,7available for the treatment of water containing dye effluents. HOAmong these methods, adsorption8 is one of the most effective NaO3S Nprocesses used for the removal of dye from waste water. N Considerable work has been done to remove toxic dyesfrom the effluents using low cost adsorbents. Some of thematerials used are apricot stone9, sugarcane bagasse10, rubber NaO3S(Hevea brasiliensis) seed coat11, neem (Azadirachta indica)leaf powder12, coir pith13, bamboo dust, coconut shell, ground- SO3Nanut shell, rice husk, straw14, orange peel15, sunflower seed Fig. 1. Molecular structure of acid red 18
220 Suresh et al. Asian J. Chem. TABLE-1 PROPERTIES OF ACID RED 18 Parameters Value Chemical name Acid Red 18 CAS number 2611-82-7 Formula weight 604.47 Ionization Basic Molecular formula C20H11N2O10S3Na3 Chromophore Monoazo Maximum wavelength 507 nm Preparation of activated carbon: Activated carbon usedin this study was prepared by chemical activation method. TheMurraya koenigii seeds (MKS) was washed several times toremove all dirt, dust and other surface impurities. The washedseeds were dried for 24 h. The dried seed was then soaked in18 N H2SO4 (sulphuric acid) in the ratio 1:2 (w/v) and kept ina muffle furnace for 12 h at 120 ºC. The carbonized materialwas finally crushed, sieved, dried and stored in plastic con-tainers. Fig. 2. SEM micrograph of prepared activated carbon (a) before dye Characterization: The surface morphology of the activated adsorption (b) After dye adsorptioncarbon prepared from Murraya koenigii seeds was studiedbefore and after dye adsorption by using scanning electron there are marked changes on the surface morphology of themicroscopy (Hitachi S3000N). The electronic structure of carbon adsorbent before and after dye adsorption. From the SEMsamples were analyzed using FT-IR (Perkin-Elmer) spectro- pictures, it is obvious that the porous nature18 of the adsorbentmeter. The measurements were carried out in the range of 4000- would have increased the possibility for the dye to be trapped450 cm-1. Carbon samples (0.33 wt %) were stirred with dry on the adsorbent.KBr (Merck, spectroscopy grade) and then pressed to form The functional groups present on the adsorbent wereappropriate tablets. confirmed by FT-IR spectra (Fig. 3). The adsorbent gives a Batch adsorption experiments: The effect of various number of absorption peaks. The peak at 3387.5 cm-1 represen-process parameters like adsorbent dosage, pH and initial dye ted bonded hydroxyl groups. A weak alkyl C-H stretching bandconcentration for the removal of acid red 18, were carried out is observed at 2931 cm-1. The peak at 1724.5 cm-1 correspondsin batch experiments in an orbital shaker at a constant speed to C=O stretching. The peak at 1621.5 and 1231 cm-1 corres-of 160 rpm. The adsorption isotherm studies were carried out ponds to C=C stretching and -SO3 stretching, respectively. Theby agitating 50 mL of dye solution of various concentrations peak observed at 1054.5 and 885.5 cm-1 could be assigned toand fixed amount of adsorbent. After agitation, the dye solutions C-O stretching vibration and C-H out of plane bendingwere separated from the adsorbent by centrifuging (Research vibration. The adsorbent exhibits reasonable anionic exchangeCentrifuge, Remi Scientific works, Mumbai) for 5 min. The capacity due to the presence of polar functional groups on thedye removal was determined spectrophotometerically (ELICO: adsorbent.SL 207) by monitoring the absorbance changes at the wave-length of maximum absorbance (507 nm). The effect of 40adsorbent dosage was studied with different adsorbent doses(25-150 mg). Kinetic experiments were carried out using a 35mechanical stirrer in the concentration range of 60-100 mg/L.The percentage dye removal was accessed using the equation 30 (C − C f ) Percentage of dye removal = i × 100 (1) Transmittance (%) Ci 25 The amount adsorbed at equilibrium qe (mg/g) was cal- 20culated by 1621.5 (C − C f )V Amount adsorbed (q e ) = i (2) 15 M 885.5where Ci and Cf are the liquid phase concentrations of the dye 1724.5 10 581.5at initial and equilibrium concentrations (mg/L), respectively,M = mass (g) of adsorbent and V = volume of dye solution (L) 5 2931 1054.5Langmuir and Freundlich isotherms were employed to study 3387.5 1231the adsorption capacity of the adsorbent. 0 4000 3500 3000 2500 2000 1500 1000 500 RESULTS AND DISCUSSION wave number (cm ) −1 Characterization of the adsorbent: Morphological study Fig. 3. FT-IR Spectra of the activated carbon prepared from Murrayaby SEM of the adsorbent shown in Fig. 2(a-b) revealed that koenigii seeds
Vol. 23, No. 1 (2011) Adsorption of Acid Red 18 onto Activated Carbon Prepared from Murraya koenigii (Curry Tree) Seeds 221 Effect of adsorbent dosage: A fixed concentration of 65 45dye (40 mg/L) was taken and the adsorbent dosage was variedin the range of 25-150 mg at a constant volume (50 mL) keeping 60all other experimental conditions constant. Amount Adsorbed (mg/g) 40 Fig. 4 shows that, an increase in adsorbent dosage increases 55 % Dye removalthe adsorption amount until a particular dosage at whichadsorption becomes constant. The increase in adsorption 50 35following an increase in adsorbent dosage can be attributed tothe availability of more adsorption sites8. However, the amount 45 30adsorbed per unit mass of the adsorbent decreases considerably. 40As the adsorption sites remain unsaturated during the adsorption % Dye Removal vs Initial dye concentrationprocess there is a decrease in unit adsorption with increasing Amount Adsorbed vs Initial dye concentration 25 35dose of adsorbent16. When the adsorbent and the solute concen- 40 60 80 100 120tration are low then the sorption rate is low. On the other hand, Initial Dye Concentration (mg/L)a high adsorbent to solute concentration ratio increases the Fig. 5. Percentage dye removal versus initial dye concentration (m = 0.05 g;rate of adsorption on the adsorbent surface and hence there is V = 0.05 L; t = 8 h)a decrease in the solute concentration in solution. Theoretically, the adsorbent has a finite capacity to absorb the 30 adsorbate and hence there is a limit beyond which no further 90 adsorption can occur20. The monolayer capacity can be repre- sented by the expression: 80 25 Q K C qe = m L e (3) 1 + K L Ce 70 % Dye removal The linear form of the above equation is represented as: qe (mg/g) 20 60 Ce 1 C = + e (4) qe QmK L Qm 50 where KL = related to the free energy of adsorption (L/mg) 15 % Dye Removal vs Adsorbent Dosage and Qm = maximum adsorption capacity. The values of Qm 40 qe vs Adsorbent dosage and KL were calculated from the slope and intercept of the linear plot (Fig. 6). The equilibrium concentration and hence 30 10 20 40 60 80 100 120 140 160 the amount of dye adsorbed were calculated by varying the Adsorbent Dosage (mg/50mL) dye concentration between 40 and 120 mg/L with a fixedFig. 4. Percentage of dye removal versus adsorbent dosage (C0 = 40 ppm; adsorbent dose and all other experimental conditions kept V = 0.05 L; t = 8 h) constant. Effect of initial dye concentration (Ci): The effect of 1.8initial dye concentration was studied by using a fixed adsorbent 1.6dosage (50 mg) for different initial dye concentrations (40,50, 60, 70, 80,100 and 120 mg/L). 1.4 From Fig. 5, it can be observed that the percentageremoval of dye decreases with the increase in initial concen- 1.2tration of dye. This is due to the saturation of the adsorption 1.0 Ce/qe (g/L)sites at higher concentrations. It is also observed that the actualamount of dye adsorbed increases with the increase in initial 0.8dye concentration (Ci). An increase in Ci increases the inter-actions between the adsorbent and adsorbate. Therefore there 0.6is an increase in the rate of adsorption of dye. 0.4 Adsorption isotherms: In accessing the equilibriumnature of adsorption of the adsorbent, three well known isotherms 0.2namely Langmuir, Freundlich and Temkin were selected for 0.0the present study. An adsorption isotherm describes the 10 20 30 40 50 60 70 80relationship between the mass of the adsorbate that is adsorbed Ce (mg/L)per unit weight on the adsorbent and the concentration of Fig. 6. Langmuir isotherm for acid red 18 adsorption onto Murraya koenigiidissolved adsorbate in the liquid phase at equilibrium. seeds Langmuir adsorption isotherm: The Langmuir adsorp-tion isotherm is based on the assumption19 that an adsorbent The isotherm constants for the Langmuir isotherm underadsorbs the dye at specific homogeneous sites and once that study were calculated from the linear form of the model andsite is occupied, no further adsorption takes place at that site. the correlation coefficients are given in Table-2.
222 Suresh et al. Asian J. Chem. TABLE-2 1.8 LANGMUIR, FREUENDLICH AND TEMKIN CONSTANTS FOR THE ADSORPTION OF ACID 1.7 RED 18 ONTO Murraya koenigii SEEDS Adsorbent Values 1.6 Langmuir 1.5 qm (mg/g) 53.19 KL (L/mg) 0.066 log qe R2 0.9992 1.4 Freundlich 1.3 KF (mg/g) 11.54 n 3.12 1.2 R2 0.9801 Temkin 1.1 KT (L/mg) 0.762 B1 11.122 1.0 R2 0.9921 1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9 log Ce An essential characteristic of Langmuir isotherm can be Fig. 7. Freundlich isotherm for acid red 18 adsorption onto MKSexpressed in terms of a dimensionless constant called the equili-brium parameter21. by Temkin and Pyzher and it is suggested that the heat of 1 adsorption and the interactions of the molecules decrease RL = × C0 (5) linearly with coverage23. The adsorption is characterized by a (1 + K L ) uniform distribution of binding energy. The Temkin equation The value of RL indicates the type of isotherm to be is given asfavourable (0 < RL < 1), linear (RL = 1), unfavourable (RL > 1) RTor irreversible RL = 0, where KL is the Langmuir constant and qe = ln(K T C e ) (8) bC0 is highest initial dye concentration (mg/L). The value of RL or, the above equation can be simplified in the linear form asis found to be in the range of 0.2747 to 0.1121 for a dye concen-tration of 40-120 mg/L indicating favourable adsorption of q e = B1 ln K T + B1 ln C e (9)acid red 18 onto MKS. where B1 = RT/b and KT is the Temkin isotherm constant (L/g) Freundlich adsorption isotherm: Freundlich isotherm where these constants can be calculated from a plot of qe versusis an empirical equation employed to describe heterogeneous ln Ce (Fig. 8) and are presented in Table-2.systems. The Freundlich equation is commonly given by: 50 q e = K F C1/n e (6) 45where qe is the amount of solute adsorbed per unit weight ofadsorbent (mg/g), Ce is the equilibrium concentration of solute 40in the bulk solution (mg/L), KF and n are Freundlich constants 35indicating the relative adsorption capacity and sorption intensityof the adsorbents (mg/g). A linear form of the Freundlich 30expression can be obtained by taking logarithms of the non- qe (mg/g) 25linear form and can be written as 20 1 log q e = log C e + log K F (7) 15 n The Freundlich constants KF and n can be calculated from 10the slope and intercept of the linear plot with log qe versus log 5Ce (Fig. 7). The Freundlich model assumes that the adsorption of the 0 2.6 2.8 3.0 3.2 3.4 3.6 3.8 4.0 4.2 4.4dye occurs on a heterogeneous surface by multilayer adsorptionwith the total adsorption increasing rapidly with an increase ln Cein concentration. Fig. 8. Temkin isotherm for acid red 18 adsorption onto Murraya koenigii seeds According to Treybal22 it has been shown using mathe-matical calculations that n values in the range of 0 < n > 1 The linear form of the Temkin equation is used to analyzerepresents favourable adsorption. The isotherm constants Kf the adsorption data and it is observed that the Temkin isothermand n were calculated from the linear form of the model and fitted in comparatively well when compared with thethe value of Kf, n and correlation coefficients are given in the Freundlich isotherm. The R2 value (0.9921) is also good whenTable-2. compared to the Freundlich isotherm which proves the appli- Temkin adsorption isotherm: The effect of indirect sorbate/ cability of Temkin isotherm for the adsorption of acid red 18adsorbate interactions on adsorption isotherms is considered on to Murraya koenigii seeds.
Vol. 23, No. 1 (2011) Adsorption of Acid Red 18 onto Activated Carbon Prepared from Murraya koenigii (Curry Tree) Seeds 223 The Langmuir, Freundlich and Temkin curve for acid red 1.418 adsorption onto Murraya koenigii seeds along with the 1.2 40 ppmexperimental data are given in Fig. 9. It is clear that the experi- 1.0 60 ppmmental data fit closely with predicted data for Langmuir adsorp- 0.8 80 ppmtion isotherm with R2 values fitting the following series; Langmuir 100 ppm 0.6> Freundlich > Temkin, for adsorption of acid red 18 on to log (qe-qt) 0.4Murraya koenigii seeds. The surface chemistry of the activatedcarbon is a key factor in interpreting the dye adsorption process24. 0.2The presence of surface oxygen groups on the carbon prepared 0.0from Murraya koenigii seeds imparts a polar character to the -0.2activated carbon surface, that provides electrostatic attraction -0.4for the preferential adsorption of anionic dye molecules on -0.6the carbon surface and hence from the results obtained it is -0.8evident that Murraya koenigii seeds could be used as an effec- 0 20 40 60 80 100 120tive low cost adsorbent for the removal of dye from aqueous t (min)solution. Fig. 10. Pseudo first order kinetics plot at four different initial concentration of acid red 18 onto Murraya koenigii seeds 45 Pseudo-second order kinetics: The pseudo second order model is given by the equation 40 t 1 t = + (11) q t K 2q 2 q t e A plot of t/qt versus t (Fig. 11) enables calculation of the qe (mg/g) 35 rate constant K2 which in turn is used to calculate the initial sorption rate h as follows: Experimental 30 Langmuir Predicted h = K 2q 2 e (12) Freuendlich Predicted Temkin Predicted 6 25 40 ppm 5 60 ppm 10 20 30 40 50 60 70 80 80 ppm Ce (mg/L) 100 ppm 4Fig. 9. Comparative fit of Langmuir, Freundlich and Temkin isotherm with t/qt (min g/mg) the equilibrium data plotted as qe versus Ce (m = 0.05 g; V = 0.05 L; t = 8 h) 3 Kinetics: Adsorption process rate can be explained by 2adsorption kinetics. It is observed that activated carbon preparedfrom Murraya koenigii seeds adsorb dyes effectively and the 1process attains equilibrium slowly with the rate of adsorptioninfluenced by the presence of functional groups such as carbo- 0 0 20 40 60 80 100 120xylic, carbonyl, hydroxyl, ether, lactone etc., on the carbon t (min)surface that tends to generate different types of adsorbent- Fig. 11. Pseudo second order kinetics plot at four different initialadsorbate interactions25. concentration of acid red 18 onto Murraya koenigii seeds Pseudo-first order kinetics: A simple kinetic analysisof adsorption, the pseudo first order kinetics and its integrated The qe values calculated from the pseudo-second orderform is given by model system are in good agreement with the experimental qe K1 values. It is observed that the K2 value decreases with increasing log (q e − q t ) = log q e − (10) 2.303t dye concentration and then increases. The correlation coeffi-where K1 is the first order rate constant that is calculated from cient (R2) of the linear plot is very high (> 0.99) for all thethe slope of the plot of log (qe - qt) versus time (Fig. 10). A concentrations studied. This indicates that the adsorption followsplot of log (qe - qt) versus time enables calculation of the rate the second order model and the adsorption process is a chemi-constant K1 and from the slope and intercept of the plot, qe (pred) sorption process. The values of kinetic constants and qe ofcan be calculated. The pseudo first order model data do not acid red 18 adsorption onto Murraya koenigii seeds are givenfall on the straight line for different initial concentrations studied, in Table-3.it is also observed that the predicted qe value and the experi- Table-4 gives the adsorption capacity of some of the lowmental qe values do not coincide and hence pseudo-first order cost adsorbents used for adsorption of dyes. From the Table-4,model is not applicable. it is seen that the adsorption ability of the carbon prepared
224 Suresh et al. Asian J. Chem. TABLE-3 KINETIC MODEL VALUES FOR THE ADSORPTION OF ACID RED 18 ON TO ACTIVATED Murraya koenigii SEEDS (MKS) Concentration qe(exp) Pseudo first order values Pseudo second order values (ppm) (mg/g) qe(calc) (mg/g) K1 (min-1) R2 qe(calc) (mg/g) K2 (g/(mg min)) h R2 40 23.06 12.67 0.03132 0.9823 24.21 0.004891 2.86 0.9989 60 28.71 14.41 0.03155 0.9950 29.94 0.004520 3.76 0.9987 80 28.86 17.15 0.02648 0.9888 30.39 0.003014 2.78 0.9979 100 31.05 18.66 0.03155 0.9818 32.78 0.003212 3.45 0.9989 TABLE-4 3. T. Robinson, G. McMullan, R. Marchant and P. Nigam, Biores. Tech., ADSORPTION CAPACITIES OF DIFFERENT 77, 247 (2001). LOW COST ADSORBENTS FOR DYE REMOVAL 4. M. Vautier, C. Guillard and J.M. Herrmann, J. Catal., 201, 46 (2001). FROM AQUEOUS SOLUTION 5. C. Allegrea, M. Maisseub, F. Charbita and P. Moulina, J. Hazard. Mater., Adsorption Reference B116, 57 (2004). Adsorbent Dye material 6. A.G. Vlyssides, M. Loizidou, P.K. Karlis, A.A. Zorpas and D. capacity (mg/g) number Papaioannou, J. Hazard. Mater., B70, 41 (1999). Orange peel Acid violet 17 19.88 15 7. P.C. Vandevivere, R. Bianchi and W. Verstraete, J. Chem. Tech. Biotech., Coir pith Acid violet 8.06 26 72, 289 (1998). Sugarcane Acid orange 10 5.78 27 8. V.K. Garg, R. Gupta, A.B. Yadav and R. Kumar, Biores. Tech., 89, 121 bagasse (2003). Rice husk Acid blue 50.00 28 Egyptian 9. E. Demirbas, M. Kobya and M.T. Sulak, Biores. Tech., 99, 5368 (2008). Acid blue 25 17.50 29 10. M. Valix, W.H. Cheung and G. McKay, Chemosphere, 56, 493 (2004). bagasse pith Egyptian 11. B.H. Hameed and F.B.M. Daud, Chem. Eng. J., 139, 48 (2008). Acid red 114 20.00 29 12. K.G. Bhattacharyya and A. Sharma, Dyes Pigm., 65, 51 (2005). bagasse pith Wood sawdust Acid blue 25 5.99 30 13. C. Namasivayam, R. Radica and S. Suba, Waste Manag., 21, 381 (2001). Murraya Present 14. N. Kannan and M.M. Sundaram, Dyes Pigm., 51, 25 (2001). Acid red 18 53.19 15. R. Sivaraj, C. Namasivayam and K. Kadirvelu, Waste Manag., 21, 105 koenigii seeds study (2001). 16. N. Thinakaran, P. Baskaralingam, M. Pulikesi, P. Panneerselvam andfrom Murraya koenigii seeds is comparatively good when S. Sivanesan, J. Hazard. Mater., 151, 316 (2008).compared with some of the low cost adsorbents already 17. M. Jambulingam, S. Karthikeyan, P. Sivakumar, J. Kiruthika andreported in the literature for the adsorption of acid dyes from T. Maiyalagan, J. Sci. Ind. Res., 66, 495 (2007).aqueous solution. The adsorption capacity of the adsorbent 18. H. Yoshida, A. Okamoto and T. Kataoka, Chem. Eng. Sci., 48, 2267 (1993).(qmax) prepared suggests that acid red 18 is comparatively easily 19. I. Langmuir, J. Am Chem. Soc., 40, 1361 (1918).adsorbed by the activated carbon used in the present study. 20. Y.C. Wang, Y.S. Szeto, W.H. Cheung and G. McKay, Langmuir, 19, 7888 (2003).Conclusion 21. Y. Bulut and H. Aydin, Desalination, 194, 259 (2006). The adsorption isotherm was best defined by the Langmuir 22. R.E. Treyball, Mass Transfer Operations, McGraw Hill, New York, edn.isotherm model and the adsorption capacity found to be 53.19 3 (1980). 23. M.J. Temkin and V. Pyzhev, Acta Physiochim. URSS, 12, 217 (1940).mg/g for the prepared activated carbon. The adsorption process 24. M.F.R. Pereira S.F. Soares, J.F.M. Orfao and J.L. Figueiredeo, Car-follows pseudo-second order model with good correlation. The bon, 41, 811 (2003).RL value (from Langmuir Isotherm Table-2) between 0 and 1 25. J.L. Figueiredo, M.F.R. Pereira, M.M.A. Freitas and J.J.M. Orfao, Car-shows favourable adsorption. The material used in this study bon, 37, 1379 (1999). 26. C. Namasivayam, M.D. Kumar, K. Selvi, R.B. Ashruffunissa, T. Vanathiis an agricultural waste product, economical to use as an alterna- and R.T. Yamuna, Biomass Bioenergy, 21, 477 (2001).tive to costlier adsorbents used for dye removal in wastewater 27. W.T. Tsai, C.Y. Chang, M.C. Lin, S.F. Chien, H.F. Sun and M.F. Hsieh,treatment processes. Chemosphere, 45, 51 (2001). 28. M.M. Mohamed, J. Colloid Interphase Sci., 272, 28 (2004). REFERENCES 29. B. Chen, C.W. Hui and G. McKay, Chem. Eng. J., 84, 77 (2001). 30. Y.S. Ho and G. McKay, Process Saf. Environ. Prot., 76, 183 (1998).1. P.K. Dutta, Indian J. Environ. Prot., 14, 443 (1994).2. K. Kadirvelu, C. Karthika, N. Vennilamani and S. Pattabhi, Chemo- sphere, 60, 1009 (2005).